Structure Irregularity Impedes Drop Roll-Oﬀ at Superhydrophobic Surfaces Simon Tylsgaard Larsen, Nis Korsgaard Andersen, Emil Søgaard, and Rafael Taboryski* Department of Micro- and Nanotechnology, Technical University of Denmark, DTU Nanotech, Building 345E, DK-2800 Kongens Lyngby, Denmark ABSTRACT: We study water drop roll-oﬀ at superhydrophobic surfaces with diﬀerent surface patterns. Superhydrophobic microcavity surfaces were fabricated in silicon and coated with 1H,1H,2H,2H-perﬂuorodecyltrichlorosilane (FDTS). For the more irregular surface patterns, the observed increase in roll-oﬀ angles is found to be caused by a decrease of the receding contact angle, which in turn is caused by an increase of the triple phase contact line of the drops for those more irregular surfaces. To understand the observation, we propose to treat the microdrops as rigid bodies and apply a torque balance between the torque exerted by the projected gravity force and the torque exerted by the adhesion force acting along the triple line on the receding side of the drop. This simple model provides a proper order of magnitude estimate of the measured eﬀects.

■

INTRODUCTION Inspired by the water-repellant properties of many plant leaves,1 artiﬁcial superhydrophobic surfaces have received much attention in the past decade.2,3 Superhydrophobicity is often achieved by applying micro- and nanostructures to a ﬂat and chemically hydrophobic surface. The surface structures will keep a drop resting on the surface in a suspended state, only touching the top of the structures. In this case, the contact angle is traditionally described in the framework of the Cassie equation4,5 and depends only on the hydrophobicity of the surface material and the fractional area of contact between the water and the solid surface. Some recent work has however stressed the importance of the conditions along the triple-phase line of the droplets resting on the surface.6 A common design for superhydrophobic surfaces is nanometer-sized, random surface roughness applied to regularly distributed, micrometersized pillars. A range of silicon microfabrication techniques have been used to fabricate surface structures,7−12 including advanced pillar structures with undercut13 and sidewall roughness.14 In many practical applications like underwater friction reduction15, and low-biofouling materials,17 water repellency is not the only important property. Also, the surfaces have to be stable in their superhydrophobic state when immersed in water. The superhydrophobic nature of the surface relies on the existence of a thin layer of air pockets between the solid surface and the liquid. If the air layer is not stable, the liquid will wet the entire surface irreversibly, resulting in a transition from the Cassie state to the so-called Wenzel state and an associated abrupt decrease in contact angle. Structures made of pillars or other protrusions are especially vulnerable to this transition, since a local collapse of the Cassie state will spread out to the remaining surface.18 In contrast, superhydrophobic surfaces © 2014 American Chemical Society

made of microcavities are relatively stable underwater due to the existence of many separate, conﬁned air pockets. However, for droplets moving across the surface, microcavity surfaces have been shown to possess diﬀerent wetting properties from pillars even for similar surface coverage.19 Microcavity surfaces have been fabricated in silicon20,21 and polymer18,22,23 with static contact angles in the same range as for pillar surfaces. Superhydrophobic surfaces are often characterized by their contact angle. In terms of water repellency though, another interesting property of the surfaces is the roll-oﬀ anglethe angle which the substrate should be tilted to make the drop roll oﬀ. This angle depends not only on the contact angle but also on the diﬀerence between the advancing and receding contact angles of the drop, the so-called contact angle hysteresis.24 In fact, surfaces can exhibit large equilibrium contact angles and still pin droplets at 90° tilting of the substrate.11 Since drop rolloﬀ is determined by the pinning of the triple-contact line of the drop,25 it must depend on the local conﬁguration of this line and thus the geometry of the surface microstructures. The pinning of the triple-contact line is caused by adhesion forces acting on the microscale by formation of capillary bridges along the triple-contact line on the receding side of the bridge.26 For superhydrophobic surfaces made of round and square pillars, it was shown that the contact angle hysteresis was larger for square pillars.27 This was explained by pinning of the drop to the sharper edges of these structures. In this paper, we present a systematic study of drop roll-oﬀ at superhydrophobic cavity surfaces with varying degree of regularity. Moreover, we provide a simple model to explain the often observed Received: February 25, 2014 Revised: April 15, 2014 Published: April 15, 2014 5041

dx.doi.org/10.1021/la5007633 | Langmuir 2014, 30, 5041−5045

Langmuir

Article

etched with a D-RIE process (STS Pegasus DRIE) to a target depth of 3.0 μm. The photoresist was removed by an oxygen plasma process (ashing), and the hydrophobicity of the structured silicon surfaces was increased by applying a monolayer of 1H,1H,2H,2H-perﬂuorodecyltrichlorosilane (FDTS) by molecular vapor deposition with an Applied Microstructures MVD 100. Three identical wafers were fabricated, and all measurements were carried out within 1 week after FDTS coating. Scanning electron microscope (SEM) images were performed with a LEO 1550 scanning electron microscope. An Attension Theta optical tensiometer was used to measure roll-oﬀ angles and contact angles. Drop volumes were always 5 μL.

relationship between contact angle hysteresis and surface structure irregularity. In this model the eﬀect is caused by adhesive forces with action predominantly along the triplecontact line on the receding side of the moving drop. Although demonstrated for cavity types of surface structures in this paper, we believe this eﬀect is general and applies to any superhydrophobic surface.

■

EXPERIMENTAL SECTION

The silicon wall structures shown in Figure 1 were fabricated from a photomask using photolithography and dry etching. A Python

■

Figure 1. SEM images of wall structures in silicon. From (a) to (d) the imposed irregularity increases, going from square-shaped wall structures to a chaotic grid of walls. Irregularity factors are (a) 0, (b) 0.4, (c) 0.8, and (d) 1.2. (e) S′ = ⟨x′⟩/x0 plotted vs the irregularity factor. ⟨x′⟩ is the average side length of the perturbed structures. The irregularity factor is deﬁned as the side length Δx0 of the square in which the points could be moved to a random position divided by the distance between points in the original array Δx0/x0.

RESULTS AND DISCUSSION Figure 1 shows SEM images of increasingly irregular wall structures starting from a regular grid with a square side length of 10 μm. Static contact angles were measured for all 14 diﬀerent surface geometries on three diﬀerent wafers, giving an average static contact angle of 158.6 ± 1.7°. For ﬂat FDTScoated areas on the same wafers over eight droplets, the contact angle was 113.7 ± 3.1°. The errors reported in our measurements are the standard deviations on each set of measurements. The increase in contact angle implies that the water drops are in the Cassie−Baxter state, only touching the top of the thin wall structures. Since the variation in static contact angle of the structured surfaces is very small, we can conclude that the static contact angle does not depend on the shape of the wall structures but rather on the surface coverage area fraction (which is constant for our surfaces) as predicted by the Cassie−Baxter equation. Next, we studied the eﬀect of pattern irregularity on the rolloﬀ angle, i.e., the angle which the surface should be tilted for the drop to roll oﬀ. While pattern irregularity has little eﬀect on the static contact angle, the eﬀect on roll-oﬀ angles is signiﬁcant. As seen from Figure 2, the angles at which a drop rolls completely oﬀ the surface (black lines) increase dramatically for more irregular structures. Also, for the smaller structures (10 μm, solid line) roll-oﬀ angles are higher than for larger structures (20 μm, dashed line). An interesting observation is made when we compare the tilting angles for complete roll-oﬀ with the angles where the drop makes its ﬁrst

program was used to deﬁne the photomask text ﬁle. First a regular square-shaped array of (x, y) points was deﬁned with side a length x0. Next, irregularity was introduced by moving each point to a random position in a square centered on this point. The level of irregularity was adjusted by increasing the side length Δx0 of the square in which the points could be moved to a random position and quantiﬁed by an irregularity factor deﬁned as the side length of this square divided by the distance between points in the original array Δx0/x0. An irregularity factor of 0 thus represents an ordered square array while 1 represents an almost completely irregular array (see Figure 1). Grids were fabricated from arrays starting with respectively x0 = 10 μm and x0 = 20 μm side length and with irregularity factors of 0.0, 0.2, 0.4, 0.6, 0.8, 1.0, and 1.2. Finally the points were connected with thin rectangles deﬁning the wall structures. The width of the walls is adjusted to ensure that the total projected area of the wall structures is constant and ranges from 400 nm for the ordered structures to 354 nm for the most irregular structures. The average length of the lines ⟨x′⟩ however increases with the irregularity factor Δx0/x0 and can readily be calculated from the photolithography mask layout ﬁle. This is shown in Figure 1e, where we calculated and plotted the quantity S′ = ⟨x′⟩/x0 . We note that S′ is an injective function of the irregularity factor. A thin layer of photoresist was applied to 4 in. silicon wafers, and the photomask pattern was transferred to the photoresist using a Canon FPA-3000 EX4-Deep UV Stepper. Next, the wafers were

Figure 2. Water drop roll-oﬀ angles plotted against the irregularity factor of the microstructured surfaces. Red lines represent the tilted angle at which the drop makes the ﬁrst sliding movement. Black lines represent the angle at which the drop rolls oﬀ the surface completely. Green lines represent complete roll-oﬀ angles for surfaces that are rotated 45° relative to the roll-oﬀ direction. Solid and dashed lines represents structures with x0 = 10 μm and x0 = 20 μm, respectively. 5042

dx.doi.org/10.1021/la5007633 | Langmuir 2014, 30, 5041−5045

Langmuir

Article

in between the two limits, ﬁrst movement and complete roll-oﬀ, calculated using eq 1. However, eq 1 only predicts the relationship between contact angle hysteresis and tilt angle but provides no explanation why contact angle hysteresis increases when the structures become more irregular. A deeper understanding of the behavior of the roll-oﬀ angles can be obtained by studying the advancing and receding contact angles of the surfaces, measured as the front and rear contact angles just before drop roll-oﬀ. Recent environmental scanning electron microscopic studies of contact line depinning from textured surfaces26 show that while the drop on the advancing side simply rolls over the surface, the receding triple-contact line is pinned to the surface by the creation of capillary bridges that exerts an adhesion force between the surface textures and the drop surface. As shown in Figure 4, this force F is eﬀectively strongest at the most rear part of the triple-contact line, where the capillary

movement (red lines, Figure 2). Clearly, the latter remain relatively constant for the diﬀerent surfaces. In other words, for the regular wall structures water drops roll oﬀ the surface completely, shortly after they make the ﬁrst movement, while for the irregular surfaces they tend to move in steps until they roll oﬀ at a larger contact angle. Probably this behavior at irregular surfaces is connected to the many possible local conﬁgurations of the triple-contact line. For the drop to roll oﬀ completely, the conﬁguration with the strongest adhesion along the triple-contact line has to be overcome. Since the more regular structures are directional of nature, we repeated the roll-oﬀ measurements with the surfaces rotated 45° relative to the previous roll-oﬀ direction (green lines, Figure 2). Regardless of rotation of the sample, we observed the same roll-oﬀ angles, suggesting that pinning of the drop takes eﬀect on a band at the perimeter of the drop, where the directional eﬀects averages out, and the important parameter is the line density per area. Clearly, complete roll-oﬀ angles are larger for the more irregular structures. The observed roll-oﬀ angles appear to be closely connected to the contact angle hysteresis and can be understood as resulting from a force balance between the projected gravity force and the projected line force acting along the triple-contact line. This relationship can be expressed in the well-known equation28 ρ NV sin α = 2γa(cos θR − cos θA)

(1) Figure 4. Graphical illustration of the model leading to eq 3. (a) Drop proﬁle recorded with the camera on the contact angle goniometer at a tilt angle. (b) Sketch showing imagined formation of capillary bridges between the drop and the surface structure at the triple phase line. (c) Sketch of the drop geometry in the roll situation; the torque associated with the adhesion force F at the triple line is balanced by the torque associated with the gravity force ρgV projected through the tilt angle α.

where ρ is the mass density of the liquid, g the acceleration of gravity, V the volume of the sessile drop, α the inclination angle of the plane on which the drop will roll, γ the surface tension of the liquid, a the radius of the apparent interface area between the drop and the substrate, and θR, θA the receding and advancing contact angles, respectively. In Figure 3 we plot the

bridge is most stretched. Because of its small size, a sessile drop is only slightly perturbed from a round shape even when the plane is tilted as seen in Figure 4a, and if we further make the approximation of treating the drop as a rigid body, we may look at the torque exerted by the adhesion force on the drop that will prevent the drop from rolling. The numerical value of this torque will be of order τ⊥ ∼ aF. The numerical value of the torque that on the other hand will roll the drop will be of order τ∥ ∼ r sin(θR − π/2)ρgV sin α, where r is the radius of the drop. We may then express the rolling condition as τ∥ > τ⊥. In order to relate the receding contact angle to the irregularity factor, we recall that the surface tension can be expressed as a force per unit of length and express the eﬀective adhesion force as the product of surface tension and some length

Figure 3. Contact angle hysteresis, plotted as the diﬀerence of the cosines of measured receding and advancing contact angles as a function the irregularity factor. The black full line shows the contact angle hysteresis calculated by eq 1 corresponding to the roll-oﬀ angles corresponding to complete roll-oﬀ, while the dashed black line is calculated using the tilt angles corresponding to the ﬁrst movement of the drops. Only data for x0 = 10 μm are shown. 2a = 726 μm is used in the calculation, corresponding to a static contact angle of 160°. The error bars for the calculated hysteresis stem from the experimental variation in the tilt angle data.

F = γ S0S′

(2)

where S0 is the characteristic length of the piece of triple-contact line along which the force eﬀectively acts, while S′ is the dimensionless relative length plotted in Figure 1e as a function of the irregularity factor. The justiﬁcation for multiplying with S′ is that the adhesion force acts through the formed capillary bridge and the longer the structure lines are, the longer will be the eﬀective piece of triple-contact line along which the bridge can attach. We should expect that S0 , within a numerical constant, is of order the radius a of the apparent interface area but considerably larger than the structure side length x0. By employing the roll condition and inserting a = r cos(θR − π/2), we can equate the torques τ∥ and τ⊥ and solve for θR to predict the critical receding contact angle at which the drop will roll:

diﬀerence of the cosines of measured receding and advancing contact angles as a function the irregularity factor for our structures together with the prediction given by eq 1. This is done using the tilt angles both for the ﬁrst movement of the drop and for the complete roll-oﬀ. We see that the data ﬁt well 5043

dx.doi.org/10.1021/la5007633 | Langmuir 2014, 30, 5041−5045

Langmuir ⎛ γ S0S′ ⎞ π θR = tan−1⎜ ⎟+ 2 ⎝ ρgV sin α ⎠

Article

irregular. Roll-oﬀ angles on the other hand increased for increasing irregularity regardless of roll-oﬀ direction. Receding contact angles decreased for increasing irregularity and could be described by a simple torque balance relationship involving the gravity force projected in the direction of motion and an adhesion force acting perpendicular to the direction of motion and acting along the rear section of the triple-contact line. This implies that an increased pinning of the triple-contact line at the rear end of the drop is responsible for larger roll-oﬀ angles at more irregular surfaces. For the regular wall structures water drops roll oﬀ the surface completely, shortly after they make the ﬁrst movement, while for the irregular surfaces they tend to move in steps until they roll oﬀ at a larger angle. This behavior at irregular surfaces is probably connected to the many possible local conﬁgurations of the triple-contact line. For the drop to roll oﬀ completely, the conﬁguration with the strongest adhesion corresponding to the longest triple-contact adhesion line has to be overcome. This work calls for a more exact theory. Such a theory would involve integration of the adhesion force from the whole interface area and take into account the capillary bridge nature of the adhesion. The eﬀective adhesion force contributing to the torque will depend on the speciﬁc micro/nano topology of the surface texture, but we expect the physics to be the same for any superhydrophobic surface chemistry and surface texture.

(3)

A somewhat similar expression but based on a force balance and leading to a diﬀerent functional dependence was recently proposed by Papadopoulos et al.29 for a pillar structure. In Figure 5, the receding and advancing contact angles are plotted

Figure 5. Receding and advancing contact angles plotted against the irregularity factor for the microstructured surfaces. The receding and advancing contact angles were measured as the front and rear contact angle of a water drop immediately before complete roll-oﬀ. The red lines are ﬁtted to receding contact angle data using the characteristic length S0 as an adjustable ﬁtting parameter in eq 3. Solid and dashed lines represents structures with x0 = 10 μm and x0 = 20 μm, where the ﬁtting parameters obtained are S0 = 163 μm, and S0 = 144 μm, respectively.

■

AUTHOR INFORMATION

Corresponding Author

*E-mail [email protected] (R.T.). Author Contributions

S.T.L. and N.K.A. contributed equally. Notes

The authors declare no competing ﬁnancial interest.

against the irregularity factor of the surfaces. While the advancing contact angles stay approximately constant around 160°, the receding contact angles decrease with increasing irregularity. This implies that the pinning of the triple-contact line at the rear end of the drop is the most important factor for drop roll-oﬀ at these surfaces. This observation can be explained by a model where the drop depins from the surface by gradual stretching and eventual snatching of capillary bridges along the triple line on the receding side of the rolling drop. In Figure 5, we show the ﬁt of the expression for the receding angle given by eq 3 to the data using S0 as an adjustable ﬁtting parameter. S′ is given by the curve in Figure 1e, while the rolloﬀ angle α is taken from the data in Figure 2, V = 5 μL, and γ = 72 mN/m. The ﬁtting results in S0 = 163 μm for the x0 = 10 μm structures, while S0 = 144 μm is obtained for the x0 = 20 μm structures. For a sessile drop of 5 μL used in the experiment, the drop radius is r ≈ 1 mm, and for a static contact angle of 160°, we get a radius of the interface area of a ≈ 363 μm, which is very roughly within a factor of 2 from the ﬁtted values for S0 . This seems consistent with the aforementioned averaging of the pinning force along the perimeter of the drop over a band that is broad enough to cancel the eﬀect of the 45° rotation.

■

ACKNOWLEDGMENTS This work is supported by the Danish National Advanced Technology Foundation (HTF) through the “Advanced Technology Project LANI” (grant 011-2011-3) and through the “Advanced Technology Platform NanoPlast” (grant 0072010-2).

■

REFERENCES

(1) Barthlott, W.; Neinhuis, C. Purity of the Sacred Lotus, or Escape from Contamination in Biological Surfaces. Planta 1997, 202, 1−8. (2) Roach, P.; Shirtcliffe, N. J.; Newton, M. I. Progess in Superhydrophobic Surface Development. Soft Matter 2008, 4, 224− 240. (3) Feng, X.; Jiang, L. Design and Creation of Superwetting/ Antiwetting Surfaces. Adv. Mater. 2006, 18, 3063−3078. (4) Cassie, A. B. D.; Baxter, S. Wettability of Porous Surfaces. Trans. Faraday Soc. 1944, 40. (5) Whyman, G.; Bormashenko, E.; Stein, T. The Rigorous Derivation of Young, Cassie-Baxter and Wenzel Equations and the Analysis of the Contact Angle Hysteresis Phenomenon. Chem. Phys. Lett. 2008, 450, 355−359. (6) Larsen, S. T.; Taboryski, R. A Cassie-Like Law Using Triple Phase Boundary Line Fractions for Faceted Droplets on Chemically Heterogeneous Surfaces RID C-9321-2011. Langmuir 2009, 25, 1282−1284. (7) Xiu, Y.; Zhu, L.; Hess, D. W.; Wong, C. P. Hierarchical Silicon Etched Structures for Controlled Hydrophobicity/Superhydrophobicity. Nano Lett. 2007, 7, 3388−3393.

■

CONCLUSION In this paper, we studied the eﬀect of microstructure geometry of superhydrophobic, cavity surfaces on water drop roll-oﬀ angles as well as receding and advancing contact angles. We observed that static and advancing contact angles remained constant over surfaces ranging from regular to completely 5044

dx.doi.org/10.1021/la5007633 | Langmuir 2014, 30, 5041−5045

Langmuir

Article

(8) Bhushan, B.; Koch, K.; Jung, Y. C. Biomimetic Hierarchical Structure for Self-Cleaning. Appl. Phys. Lett. 2008, 93, 093101− 093101. (9) Chen, M.; Hsu, T.; Chuang, Y.; Tseng, F. Dual Hierarchical Biomimic Superhydrophobic Surface with Three Energy States. Appl. Phys. Lett. 2009, 95, 023702−023702. (10) Sun, G.; Gao, T.; Zhao, X.; Zhang, H. Fabrication of Micro/ Nano Dual-Scale Structures by Improved Deep Reactive Ion Etching. J. Micromech. Microeng. 2010, 20, 075028−075028. (11) Winkleman, A.; Gotesman, G.; Yoffe, A.; Naaman, R. Immobilizing a Drop of Water: Fabricating Highly Hydrophobic Surfaces That Pin Water Droplets. Nano Lett. 2008, 8, 1241−1245. (12) Kim, H.; Lee, C.; Kim, M. H.; Kim, J. Drop Impact Characteristics and Structure Effects of Hydrophobic Surfaces with Micro- and/or Nanoscaled Structures. Langmuir 2012, 28, 11250− 11257. (13) Wang, J.; Liu, F.; Chen, H.; Chen, D. Superhydrophobic Behavior Achieved from Hydrophilic Surfaces. Appl. Phys. Lett. 2009, 95, 084104−084104. (14) Lee, C.; Kim, C. Maximizing the Giant Liquid Slip on Superhydrophobic Microstructures by Nanostructuring Their Sidewalls. Langmuir 2009, 25, 12812−12818. (15) Voronov, R. S.; Papavassiliou, D. V.; Lee, L. L. Review of Fluid Slip Over Superhydrophobic Surfaces and Its Dependence on the Contact Angle. Ind. Eng. Chem. Res. 2008, 47. (16) Choi, C.; Ulmanella, U.; Kim, J.; Ho, C.; Kim, C. Effective Slip and Friction Reduction in Nanograted Superhydrophobic Microchannels. Phys. Fluids 2006, 18, 087105−087105. (17) Marmur, A. Underwater Superhydrophobicity: Theoretical Feasibility. Langmuir 2006, 22, 1400−1402. (18) Salvadori, M. C.; Cattani, M.; Oliveira, M. R. S.; Teixeira, F. S.; Brown, I. G. Design and Fabrication of Microcavity-Array Superhydrophobic Surfaces. J. Appl. Phys. 2010, 108, 024908−024908. (19) Priest, C.; Albrecht, T. W. J.; Sedev, R.; Ralston, J. Asymmetric Wetting Hysteresis on Hydrophobic Microstructured Surfaces. Langmuir 2009, 25, 5655−5660. (20) Bobji, M. S.; Kumar, S. V.; Asthana, A.; Govardhan, R. N. Underwater Sustainability of the “Cassie” State of Wetting. Langmuir 2009, 25, 12120−12126. (21) Pietsch, T.; Gindy, N.; Fahmi, A. Nano- and Micro-Sized Honeycomb Patterns through Hierarchical Self-Assembly of MetalLoaded Diblock Copolymer Vesicles. Soft Matter 2009, 5, 2188−2197. (22) Huang, Y.; Wu, J.; Yang, S. Direct Fabricating Patterns Using Stamping Transfer Process with PDMS Mold of Hydrophobic Nanostructures on Surface of Micro-Cavity. Microelectron. Eng. 2011, 88, 849−854. (23) Rasilainen, T.; Kirveslahti, A.; Nevalainen, P.; Suvanto, M.; Pakkanen, T. A. Controlling the Movement of Water Droplets with Micro- and Hierarchical Micro/nanostructures. Surf. Rev. Lett. 2011, 18, 209−222. (24) McHale, G.; Shirtcliffe, N.; Newton, M. Contact-Angle Hysteresis on Super-Hydrophobic Surfaces. Langmuir 2004, 20, 10146−10149. (25) Choi, W.; Tuteja, A.; Mabry, J. M.; Cohen, R. E.; McKinley, G. H. A Modified Cassie-Baxter Relationship to Explain Contact Angle Hysteresis and Anisotropy on Non-Wetting Textured Surfaces. J. Colloid Interface Sci. 2009, 339, 208−216. (26) Paxson, A. T.; Varanasi, K. K. Self-Similarity of Contact Line Depinning from Textured Surfaces. Nat. Commun. 2013, 4, 1492. (27) Cansoy, C. E.; Erbil, H. Y.; Akar, O.; Akin, T. Effect of Pattern Size and Geometry on the Use of Cassie-Baxter Equation for Superhydrophobic Surfaces. Colloids Surf., A 2011, 386, 116−124. (28) Furmidge, C. Studies at Phase Interfaces. 1. Sliding of Liquid Drops on Solid Surfaces and a Theory for Spray Retention. J. Colloid Sci. 1962, 17, 309. (29) Papadopoulos, P.; Mammen, L.; Deng, X.; Vollmer, D.; Butt, H. How Superhydrophobicity Breaks Down. Proc. Natl. Acad. Sci. U. S. A. 2013, 110, 3254−3258.

5045

dx.doi.org/10.1021/la5007633 | Langmuir 2014, 30, 5041−5045